O R I G I N A L A R T I C L E
The influence of moisture content variation on
fungal pigment formation in spalted wood
, Sara C Robinson and Paul A Cooper
Eight fungal species known to produce wood pigmentation were tested for reaction to various moisture contents in two hardwood species. Fungal pigmentation byTrametes versicolorandXylaria polymorphawas stimulated at low water concentrations in bothAcer saccharum(sugar maple) andFagus grandifolia(American beech), whileInonotus hispidusandPolyporus squamosuswere stimulated above 22-28% and 34-38% moisture content in beech and in sugar maple respectively.Fomes fomentariusandPolyporus brumalisproduced maximum pigmentation in beech at 26 - 41% and in sugar maple at 59 - 96% moisture content. The pink stainingScytalidium cuboideumpigmented both wood species at above 35% moisture content. This research indicates that controlling the moisture content values of wood substrates can stimulate the intensity of pigmentation of specific fungi when spalting wood for decorative and commercial purpose.
Keywords:Fungal melanin, Pigment, Moisture content, Spalting
Spalted wood is considered a value added product and can be produced by selected fungal inoculation of the wood substrate to create unique patterns (Robinson et al. 2007), and its considerable artistic and economic value is already established (Nicholls 2002; Donovan and Nicholls 2003a,b). The main characteristics of spalting are the spatial barrier demarcation of the fungal colonies by black pigment deposition, and the distinct colored zonation (Figure 1). The black pigment is a melanin type pigment (Butler and Day 1998) and it has a protective role against unfavorable environmental conditions (Campbell 1934; Pearce 1991; Henson et al. 1999). The stained wood of various colors is an effect of secondary metabolites in the form of pigmented fungicides, produced in the wood substrate by specific fungi (Margalith 1992; Duran et al. 2002). Wood moisture content (MC) is one of the most important conditions that influence fungal behavior and wood colonization patterns (Boddy 1983b). It is established that optimal fungal growth is achieved at 35–50 % MC on a dry weight basis, with a minimum required of 20–30 % necessary for fungal development; the values vary for different fungal species and inhabited wood substrates
(Cartwright and Findlay 1958; Rayner and Todd 1979). Cartwright and Findlay (1958) also mention the ability of some fungal mycelium to survive below the fiber satu-ration point moisture content (26- 27% of the dry weight for most wood species), while spores, as well as mycelium of several fungal species, can survive for many years in dry condition (Schmidt 2006). Very high wood moisture content also inhibits fungal activity in wood substrate by limiting the quantity of the oxygen available in wood, preventing degradation (Cartwright and Findlay 1958; Boddy 1983a,b).
Moisture content of the substrate is not entirely dependent on the environmental conditions. It is known that wood-inhabiting fungi can influence the microcli-matic regime in dead wood. Some fungi are able to regu-late the moisture content of a substrate to ensure the optimal water availability, or as a strategy in antagonistic reactions, to create an environment stressful for fungal competitors, thereby avoiding combative exclusion (Boddy and Heilmann-Clausen 2008). Miller (1932) demonstrated that wood decomposer fungi like Serpula lacrymans (Wulfen) J. Schröt., Schizopora paradoxa (Schrad.) Donk andConiophora puteana(Schumach.) P. Karst., could regulate the water content of the colonized habitat. During the initial stages of colonization, the dry conditions are improved for optimal growth by the mean
Faculty of Forestry, University of Toronto, 33 Willcocks Street, Toronto M5S 3B3, Canada
of cellulose and polysaccharide decomposition, while at higher levels of humidity the water surplus is extracted from wood substrate into aerial mycelium, to ensure the optimal moisture content. By virtue of pigmented zon-ation lines that they produce, fungi fromXylariaspecies seem to maintain wood drier than ambient conditions (Boddy et al. 1989; Heilmann-Clausen 2001), while Ar-millaria species occupy wood wetter than ambient (Lopez-Real and Swift 1975; Chapela and Boddy 1988). As reported by Humar et al. (2001), moisture content of wooden blocks inoculated with Trametes versicolor (L.) Lloyd rose from 10 % to 57 % above the fiber saturation point after 12 weeks of exposure to decay, and oppor-tunistic mold fungi likePenicilliumspp. can ensure fun-gal succession on various wood substrates by improving moisture content in decayed wood (Dix 1985). However, various water content levels determine the prevalence of fungal species inhabiting the wood substrate. Based on the moisture content preference, Käärik (1974) indicate three distinctive groups that colonize wood: fungi that occupy wood at 37 –47 % moisture content, fungi that prefer a drier part of the wood of 17-23% MC, and fungi that had no restriction in terms of water availability.
There are 44 species of basidiomycetes and 10 species of ascomycetes that have been reported to form dark zone lines (Lopez-Real and Swift 1975). Research by Hu-bert(1924) indicated that fungal melanin deposition in spatial demarcation could be triggered by limited water availability. The anticipation of desiccation might cause fungal species like Xylaria polymorpha (Pers.) Grev., Bjerkandera adusta(Willd.) P. Karst.,Phellinus igniarius (L.) Quél. and Porodaedalea pini (Brot.) Murrill to de-velop an effective strategy to ensure the survival of the colonies. They produce high resistance, melanin-type
pigment that surrounds the fungal community like a barrier, blocking the water exchange within the wood substrate. This may appear as fine delimitation lines in section. Campbell (1933), in his study on zone line for-mation by X. polymorpha, refers to desiccation as the cause of a particular kind of zone lines, as well as for Ar-millaria mellea(Vahl) P. Kumm (Campbell 1934).
Laboratory studies by Lopez-Real and Swift (1975, 1977) indicate that melanized mycelium formation byA. mellea and Stereum hirsutum (Willd.) Pers., is consid-ered as a normal morphogenetic process, and occurs at any moisture content when growth is possible, except for S. hirsutumat low humidity (< 35% MC), when pig-mentation is inhibited at early stages of growth. Studies by Campbell (1933,1934), Lopez-Real (1975), Rayner and Todd (1979), Boddy (1986), and Boddy et al. (1989) de-scribe the formation of melanized mycelium in zone lines, in inter- and intraspecific antagonistic reactions, and offer a perspective on substrate and environmental conditions that influence such formations in natural set-tings. Lopez-Real and Swift (1975) indicated the exist-ence of a relationship between the moisture content of the substrate during the initial period of colonization and the ability ofArmilaria melleato form melanin.For Stereum hirsutum, only high moisture content of the substrate may be a critical factor determining pigment formation. Campbell (1933,1934) studied in vitro zon-ation of A. mellea and X. polymorpha, mentioning that optimum moisture is necessary to produce pigmenta-tion; however no specific values were indicated. Rishbeth (1951) studied the behavior of Heterobasidion annosum (Fr.) Bref. indicating that infection is critical in freshly cut stumps. Hopp (1938) investigated pigmentation of Ganoderma applanatum (Pers.) Pat. and Phellinus
igniarius (L.) Quél. and found that moisture content strongly influences the antagonistic reactions with pig-ment production in wood. However, research under la-boratory conditions is limited, and a more elaborate and consistent investigation was necessary to determine the optimal conditions for pigmentation for given wood spe-cies by fungal spespe-cies utilized in spalting. This study investigates the direct influence of moisture content of specific wood substrates on fungal pigmentation, and the results are important for manipulating fungal pig-mentation for spalting production. The ability to ma-nipulate fungal reactions through moisture content changes in wood, offers a chance to enhance the pig-mentation intensity and patterns currently available with spalted woods. It also offers an opportunity to add con-siderable value to underutilized hardwood species.
Material and Methods
Wood and fungal species selection
Two common wood species from southern Ontario, sugar maple (Acer saccharum Marsh) and beech (Fagus grandifolia L.) were selected for testing, based on their contrasting natural spalting prevalence. The average oven-dry specific gravity (SG) of the tested wood species was SG=0.68 for sugar maple and SG=0.74 for beech.
Eight fungal species were selected based on their spalt-ing ability (Table 1). The ascomycete X. polymorpha is known to produce melanin by a polyketide pathway and the basidiomycete T. versicolor probably produces mel-anin by the catechol pathway (Bell and Wheeler 1986; Taylor et al. 1988). For those fungi, we tested three strains each to determine whether melanin production varied significantly within a species. X. polymorpha strains UAMH 11518, UAMH 11519, UAMH 11520 had been isolated fromAcer saccharumin Alberta, MI, USA. TwoT. versicolor strains were obtained from the Forest
Products Laboratory in Madison, WI, USA: Mad 697 was, isolated from a cankered area of Fagus grandifolia in Vermont, USA, and strain R105 was isolated from a dead branch ofMalus sp. in New York, USA. The third strain UAMH 11521 was isolated fromAcer saccharum in Houghton, MI, USA.
Other fungal species, one strain per species, were used for additional experiments:Polyporus squamosus(Huds.) Fr. UAMH 11653 isolated from beech in Toronto, ON, Canada, Polyporus brumalis (Pers.) Fr. UAMH 11652 isolated from unidentified dead wood in Toronto area, ON, Canada, Fomes fomentarius (L.) J.J. Kickx UAMH 11654 isolated from birch in Toronto, ON, Canada, Ino-notus hispidus(Bull.) P. Karst. F2037 of unknown origin, Piptoporus betulinusUAMH 11651 (Bull.) P. Karst., iso-lated from sugar maple in Toronto, ON, Canada. One staining fungus investigated for pigment formation was Scytallidium cuboideum (Sacc. & Ellis) Sigler & Kang UAMH 4802 isolated from Na-pentachlorophenate-dipped red oak lumber.
Fungal cultures used for inoculation were grown on 95x15 mm Petri dishes with 2% malt extract agar at room temperature for two weeks prior inoculation.
Moisture content test preparation
The moisture content test was performed using a modi-fied decay jar test with vermiculite instead of soil, as out-lined in Robinson et al. (2009, 2012), to avoid eventual influence of soil substrates on pigment formation. Jars with plastic lids (250 ml) were prepared with 15g ver-miculite and variable amounts of distilled water per set. According to AWPA (2009) Standards, the amount of water added in the jars should be 130% of the water-holding capacity (WHC) of the substrate, in our case vermiculite, for optimum condition of decay. Based on vermiculite WHC, our calculations indicate that 30g of distilled water should be added in each cultured jar for standard incubation conditions. Nine levels of water availability was tested, modifying the amount of water added to each jar, in increments of 5g, five levels under and three levels above the standard conditions for decay (5g, 10g, 15g, 20g, 25g, 30g, 35g, 40g, and 45g).
Inoculation and incubation
Culture jars with vermiculite and the specified amount of distilled water were autoclaved for 30 minutes at 121°C. Five replicates per set of 14 mm wood cubes, preconditioned at 50°C to provide an initial dry weight, were surface steam sterilized for 30 minutes under at-mospheric pressure at 100°C. After cooling, the wood samples were placed in culture jars, and inoculated with a 0.5x2 cm strip of fungal inoculum. Culture jars were incubated at 27°C ± 2°C and 80% ± 5% relative Table 1 Wood and fungal species selection
Wood species/specific gravity (SG)
Fungal species/Culture collection number
Sugar maple/SG=0.68 Xylaria polymorpha UAMH 11518 UAMH 11519 UAMH 11520 Beech/SG=0.74 Trametes versicolor Mad 697
FP 72074-R UAMH 11521
Polyporus squamosus UAMH 11653
Polyporus brumalis UAMH 11652
Fomes fomentarius UAMH 11654
Inonotus hispidus F2037
Piptoporus betulinus UAMH 11651
humidity in the inoculation chamber, for eight weeks for T. versicolor and F. fomentarius and ten weeks for the remaining fungi. At the end of the period of incu-bation, blocks were removed from jars, gently cleaned at surface to remove mycelium and any traces of ver-miculite, and weighed before and after overnight oven drying to determine final moisture content and mass loss. To avoid changes of fungal pigment colors, the drying temperature was modified to 50°C instead of 103°C standard for MC testing.
Dried wood samples were scanned externally and intern-ally with Epson WorkForce 500 scanner at 2400 dpi. The obtained images were analyzed for pigment evalu-ation with Scion Image software, following the protocol described in Robinson et al.(2009a).
To analyze the importance of moisture content for fungal pigment formation, a one-way ANOVA was run, followed by Tukey’s HSD atα= 0.05, using SAS, version 9.2, with fungal inoculation and induced conditions as independent variables, for each wood species.
Estimation of initial conditions and changes of substrate moisture content
To estimate the wood moisture content in conditions simulated in the experiment, two sets of tests were run for eight weeks, without fungal inoculation, under iden-tical conditions as the main test. Five replicates of wood samples per treatment, initially oven-dried conditioned, were weighed every day for the first week and once every week for the following period, to monitor changes of moisture content in wood samples. To minimize mold contamination, wood samples were manipulated and weighted in a sterile laminar flow hood. However, for comparison, wood samples from a second set were kept in sterile conditions and weighed only at the end of the eight-week incubation period. Wood moisture content was calculated based on the final oven-dry weight.
Periodical measurement of beech and sugar maple sam-ples kept in culture conditions without fungal inocula-tion, showed that after one day, wood samples attained 70% of the final moisture content measured at the end of eight weeks; after four days, samples reached approxi-mately 80% of the final moisture content, and after ap-proximately two weeks, wood samples reached moisture content equilibrium (Figure 2). There are clear differ-ences among treatments at every stage of testing period.
Comparisons between the final results of wood samples exposed to the same moisture content settings, but kept in sterile and unsterile conditions, indicate a slightly
positive difference in water uptake of the sterile wood samples, that might be explained by water loss due to periodic handling for weight measurements. Also, the results indicate that sugar maple’s hygroscopic capacity was greater than that of beech, for the same amount of water availability (Table 2).
None of the treatments significantly influenced mass loss in beech and sugar maple. However, lower levels of moisture content attained by treatment with 5, 10 and 15 g of water resulted in stimulation of mass loss in beech inoculated with X. polymorpha, P. brumalis and P. betulinus (Figure 3a). Mass loss induced by F. fomentarius was greater in beech samples, while the rest of the fungi degraded sugar maple samples more (Figure 3a and b).
Influence of induced condition on pigment formation
External black to dark brown pigmentation byT. versico-lor (average of three strains) was higher with the low water availabilities with maximum pigmentation at treat-ment with 10 g of water for sugar maple and 15 g water for beech; these treatments resulted in similar initial conditions of approximate 30 % moisture content for
both wood species tested. Internal pigmentation in sugar maple was also stimulated by low water content. The large standard deviations for the degree of pigmentation (Figure 4) reflect the high variability among the strains used for the moisture content experiment.
External zone lines and black pigmentation produced byX. polymorpha(average of three strains) in beech and sugar maple was significant at treatments with 10 and 15 g of water for both wood species (P<0.0001). Internal pigmentation was highest in sugar maple at low mois-ture content (Figure 5). UnlikeT. versicolor, this fungus demonstrated smaller deviations among the data and a greater consistency in pigment formation among the three strains.
In the case ofI. hispidusand P. squamosus, there was no significant moisture content treatment condition that enhanced pigmentation; however, there was a tendency of enhanced dark brown pigmentation observed at higher levels of moisture content (Figures 6 and 7).
Polyporus brumalis had significant black external pig-mentation in sugar maple at treatments with 45g of water (P<0.0001), while in beech the pigmentation was stimulated at lower levels of moisture content. The same tendency was observed for F. fomentarius (Figures 8 and 9). Piptoporus betulinus, the only brown rot fungus investigated, produced no pigmentation in either wood species tested.
The red stain fungus S. cuboideum had significant external pigmentation at treatments with 20 g of water for both wood species tested (P<0.0001) at eight weeks of incubation, and there was also significant internal pigmentation in sugar maple (P<0.0001) at the same treatment (Figure 10).
For commercial and artistic purposes, spalting should result in a high intensity of wood pigmentation, while minimizing the loss in strength and integrity of the wood after exposure to fungal activity. The natural wood resistance to decay is influenced by many other factors such as wood extractives and ambient temperature. In our tests, wood integrity was reflected by mass loss mea-surements at the end of period of incubation. As expected, based on the specific gravity of the wood spe-cies tested, sugar maple samples proved to have higher degradability than beech, with few exceptions. Polyporus brumalis andS. cuboideum degraded both wood species at the same rate, andF. fomentarius was more effective for beech degradation, within the same treatments of water availability. However, sugar maple is more prone to spalting, as the occurrence of fungal pigmentation and zone line is much higher than in beech.
The moisture content in wood substrates can fluctuate considerably, and is influenced by the relative humidity Table 2 Final moisture content in wood samples (five replicates per set) incubated with various fungal species: tv =T. versicolor(average of three strains); xp =X. polymorpha(average of three strains);ih =I. hispidus; pbr =P. brumalis; pbt =P. betulinus;ff =F. fomentarius; psq =P. squamosus; sc =S. cuboideum; - = no fungal inoculation
Fungal species tv xp ih pbr pbt ff psq sc
-Treatment g water/jar Mean % moisture content /standard deviation
Beech 5 27 /5 21 /2 23 /5 27 /3 31 /2 27 /3 25 /5 13 /4 21 /3
10 34 /4 33 /4 32 /4 33 /3 31 /2 31 /2 30 /2 23 /10 25 /3
15 37 /6 35 /3 34 /5 37 /4 38 /4 34 /8 33 /5 33 /3 29 /3
20 39 /3 40 /6 44 /5 41 /2 40 /3 43 /4 40 /5 43 /4 37 /4
25 45 /8 43 /6 50 /6 44 /4 53 /3 53 /7 51 /7 46 /5 40 /4
30 46 /7 49 /5 54 /7 44 /2 52 /3 56 /4 58 /5 47 /3 50 /3
35 50 /10 50 /5 55 /5 45 /8 55 /9 52 /7 58 /14 47 /3 56 /4
40 58 /11 54 /5 58 /2 55 /6 53 /5 52 /11 62 /13 47 /5 59 /4
45 63 /14 60 /6 79 /8 59 /9 62 /2 77 /16 88 /10 49 /5 59 /3
Sugar maple 5 24 /5 23 /3 19 /4 29 /3 18 /7 8 /3 24 /1 9 /4 19 /4
10 33 /5 31 /3 33 /3 33 /5 35 /3 10 /2 29 /1 15 /1 22 /2
15 37 /6 39 /8 36 /6 36 /3 46 /2 13 /2 31 /4 20 /3 31 /2
20 41 /4 46 /3 66 /11 52 /6 66 /3 23 /4 34 /3 25 /2 36 /2
25 47 /7 51 /3 71 /9 59 /6 80 /8 24 /6 43 /2 25 /4 44 /2
30 47 /6 56 /5 77 /5 72 /4 91 /5 37 /6 44 /4 31 /4 59 /13
35 55 /6 57 /5 81 /9 82 /3 95 /6 47 /5 45 /4 37 /5 70 /11
40 76 /8 71 /7 89 /7 85 /2 96 /7 53 /3 48 /2 37 /3 82 /6
of the microclimate, the substrate hygroscopicity, and fungal decomposition activity (Chapela and Boddy 1988; Boddy et al. 1989; Heilmann-Clausen 2001; Boddy and Heilmann-Clausen 2008). From the analysis of moisture content of wood samples exposed to the same testing condition, without fungal inoculation, it was determined that sugar maple was more hygroscopic than beech (Figure 2), suggesting higher hemicelluloses, lower lignin and/or lower extractive content (Rowell 2012). For the present study, it was also important to establish the pre-dicted value of the initial moisture content that the wood substrate was able to achieve for each treatment (see Table 2).
Due to periodic removal of wood samples for weighing, the measured MC of the wood samples varied over the
experiment period. This variation could be explained either by loss of moisture through evaporation, or by changes to the position of the wood samples in the vermiculite. However, comparison of final results of this experiment with another set of sterile wood samples, kept in the same condition and measured only for final moisture content after eight weeks, indicates that the final MC of the two sets of wood samples are comparable (results not shown).
The most favorable condition for the growth of fungi in wood is slightly above the fiber saturation point (FSP: 25-30% MC), when free diffusion of enzymes can take place within the film of liquid water that coat the cell walls, but where some air spaces remain for gas diffusion (Cartwright & Findlay 1958). According to Lopez-Real
0 5 10 15 20 25 30
tv xp ih pbr pbt ff psq sc
mean % mass loss
fungal species in beech
5 10 15 20 25 30 35 40 45
AAAAAA BB B B B C BA A A A A A A
AAA A A AA A A BA BC C CCCCC
A BA BC D D DC DC DC DC B B B A A A A
A A A A A A A A BA BA B A A A A A A B B C 0 5 10 15 20 25 30
tv xp ih pbr pbt ff psq sc
mean % mass loss
fungal species in sugar maple
5 10 15 20 25 30 35 40 45 B C A BA BA BA BA BA BA C A B B BA BA BA
BABA BAABABA BA A B B A BA BA B B B B B B A DCC B B BA BABA A A A A A A A A A A BA BA BA BA BA BA BA BA BA BA A B B B D BC C
and Swift (1975), the formation of black pigmented de-limitation zones requires a similar situation, where free water still exists in the lumina of the wood cells, and the levels of concentration of CO2 are above atmospheric
conditions, with the presence of atmospheric levels of oxygen at least for the initial exposure.
However, the present study shows that the reaction of fungal species investigated at different values of water availability varied considerably, even between the two wood species studied. Trametes versicolorproduced pig-mentation at a lower moisture content equivalent of 18– 35 % for sugar maple, and 26–32 % for beech (Figure 4), with no inhibition of mass loss. The ascomyceteX. poly-morpha preferred a moisture content that was more
consistent between the two wood species studied, produ-cing maximum pigmentation at 29–33 % in sugar maple and 29–32 % initial moisture content in beech (Figure 5). However, the same moisture content that stimulated pigmentation in beech, also resulted in the highest mass loss (Figure 3a). In the case ofI. hispidus the pigmenta-tion was inhibited at low moisture contents, under 22-28% in beech and 34-38% in sugar maple (Figure 5), and no treatment had a significant influence on mass loss. The same trend can be recognized in P. squamosus (Figure 7), while F. fomentarius and P. brumalis both show a completely different tendency, with maximum pigmentation in beech at 26–41 % and in sugar maple at 59- 96% (Figures 8 and 9). The pink staining fungus
Figure 5Pigment production in beech (b) and sugar maple (sm) byXylaria polymorpha(average of three strains) at various moisture content values in ten weeks of incubation: ezl–external zone lines; ep–external pigmentation; izl–internal zone lines; ip–internal pigmentation.Error bars represent one standard deviation of five replicates per set. Different letters represent significant differences atα= 0.05 within each category.
Figure 6Pigment production in beech (b) and sugar maple (sm) byInonotus hispidusat various moisture content values in eight weeks of incubation: ezl–external zone lines; ep–external pigmentation; izl–internal zone lines; ip–internal pigmentation.Error bars represent one standard deviation of five replicates per set. Different letters represent significant differences atα= 0.05 within each category.
Figure 7Pigment production in beech (a) and sugar maple (b) byPolyporus squamosusat various moisture content values in eight weeks of incubation: ezl–external zone lines; ep–external pigmentation; izl–internal zone lines; ip–internal pigmentation.Error bars represent one standard deviation of five replicates per set. Different letters represent significant differences atα= 0.05 within each category.
S. cuboideum developed more pigmentation at an the initial moisture content above 35 % for both wood spe-cies (Figure 10). The differences in the reaction among fungal species to various moisture contents might be the outcome of fungal specificity to certain conditions and substrate constraints, as part of successional colonization that ensure wood decomposition (Boddy 1983a; Boddy and Rayner 1983; Cooke and Rayner 1984; Boddy 1986; Rayner 1986; Boddy et al. 1989). It is also known that many of the studied fungi produce different types of black pigmentation, using various phenolic compounds from wood substrates as precursors for melanin biosyn-thesis (Bell and Wheeler 1986; Butler et al. 2001). Those cumulative observations emphasize once more the com-plex interactions of fungal species in wood decay.
This research indicates that spalting could be stimu-lated by controlling moisture content of the substrate, and optimal conditions are specific to wood and fungal species. Pigmentation was stimulated at low water con-centrations in the case of T. versicolor and X. polymor-pha for both wood species tested, while I. hispidus, P. squamosus,P. brumalisandS. cuboideumshowed a ten-dency of enhanced pigmentation at higher levels of moisture content (35%-55%). Moisture content amounts tested did not significantly affect wood mass loss.
For direct applicability in industrial spalting produc-tion, fungal strains used in production should be carefully tested to assess the maximum pigmentation ability in regard with MC. Pairing of fungal strains should be considered based on their similarity of Figure 9Pigment production in beech (a) and sugar maple (b) byPolyporus brumalisat various moisture content values in eight weeks of incubation: ezl–external zone lines; ep–external pigmentation; izl–internal zone lines; ip–internal pigmentation.Error bars represent one standard deviation of five replicates per set. Different letters represent significant differences atα= 0.05 within each category.
pigment production at proximate MC values. A special consideration should be given to fungi like X. polymor-pha that produce maximum pigmentation at lower values of MC, and proved to be more consistent in strain variation. To overcome the limited surface that fungi can inhabit at low water availability due to restrained growth, a MC optimal for growth should be initially induced, followed by a drying period to stimulate pigmentation.
MC: Moisture content; WHC: Water-holding capacity.
The authors declare that they have no competing interests.
The research was financially supported by the Natural Resources of Canada (Value-to-Wood Program).
Received: 4 December 2012 Accepted: 5 December 2012 Published: 17 December 2012
American Wood Protection Association (2009) E10-06. Standard method of testing wood preservatives by laboratory soil-block cultures. AWPA Book of Standards, Birmingham, AL
Bell AA, Wheeler MH (1986) Biosynthesis and function of fungal melanins. Ann Rev Phytopathol 24:441–451
Boddy L (1983a) Effect of temperature and water potential on growth rate of wood-rotting basidiomycetes. Trans Br Mycol Soc 80:141–149 Boddy L (1983b) Carbon dioxide release from decomposing wood: effect of
water content and temperature. Soil Biol Biochem 15:501–510
Boddy L (1986) Water and decomposition processes in terrestrial ecosystems. In: Ayres PG, Boddy L (eds) Water, Fungi and Plants. Cambridge University Press, Cambridge, pp 375–398
Boddy L, Owens EM, Chapela IH (1989) Small scale variation in decay rate within logs one year after felling: effect of fungal community structure and moisture content. Fed Eur Microbiol Soc 62:173–184
Boddy L, Heilmann-Clausen J (2008) Basidiomycete community development in temperate angiosperm wood, In: Boddy L, Frankland JC, West P (eds) Ecology of Saprotrophic Basidiomycetes. British Mycological Society Symposia Series, Academic Press 28:211–237
Boddy L, Rayner ADM (1983) Origins of decay in living deciduous trees: the role of moisture content and reappraisal of the expanded concept of tree decay. New Phytol 94:623–641
Butler MJ, Day AW (1998) Fungal Melanins: a Review. Can J Microbiol 44:1115–1136 Butler MJ, Day AW, Henson JM, Money NP (2001) Pathogenic Properties of
Fungal Melanins. Mycol 93(1):1–8
Campbell AH (1933) Zone lines in plant tissue. I. The black zones formed by
Xylaria polymorpha(Pers.) Grev. in hardwoods. Ann Appl Biol 20(1):123–145 Campbell AH (1934) Zone lines in plant tissue. II. The black zones formed by
Armillaria mellea(Vahl)Quel. Ann Appl Biol 21:1–22
Cartwright KSTG, Findlay WPK (1958) Decay of timber and its prevention. HMSO, London
Chapela IH, Boddy L (1988) Fungal colonisation of attached beech branches, II. Spatial and temporal organization of communities arising from latent invaders in bark and functional sapwood under different moisture regimes. New Phytol 110:47–57
Cooke RC, Rayner ADM (eds) (1984) Ecology of saprotrophic fungi. Longman, London
Dix NJ (1985) Changes in relationship between water content and water potential after decay and its significance for fungal successions. Trans Br Mycol Soc 85:649–653
Donovan GH, Nicholls D (2003b) Estimating consumer willingness to pay a price premium for Alaskan secondary wood products. Gen. Tech. Note. PNW:RP-553. USDA Forest Serv., Pacific Northwest Res. Sta, Portland, OR
Donovan G, Nicholls D (2003a) Consumer preferences and willingness to pay for character-marked cabinets from Alaska birch. Forest Prod J 53(11/12):27–32
Duran N, Teixeira MFS, De Conti R, Esposito E (2002) Ecological-friendly pigment from fungi. Cr Rev Food Sci Nutr 42:53–66
Heilmann-Clausen J (2001) A gradient analysis of communities of macrofungi and slime moulds ondecaying beech logs. Mycol Res 105:575–596 Henson JM, Butler MJ, Day AW (1999) The Dark Side Of The Mycelium: Melanins
of Phytopathogenic Fungi. Ann Rev Phytopathol 37:447–471
Hopp H (1938) The formation of coloured zones by wood-destroing fungi in culture. Phytopathol 28:601–620
Hubert EE (1924) The diagnosis of decay in wood. Agr Res J 29(11):523–569 Humar M, Petric M, Pohleven F (2001) Changes of the pH value of impregnated
wood during exposure to wood-rotting fungi. Holz Roh-Werkstoff 59:288–293 Käärik (1974) Decomposition of wood. In: Dickinson CH, Pugh GJF (eds) Biology
of Plant Litter Decomposition. Academic Press, London, p 129 Lopez-Real JM (1975) Formation of pseudosclerotia (‘zone lines’) in wood
decayed byArmillaria melleaandStereum hirsutum.I. Morphological aspects. Trans Br Mycol Soc 64:465–471
Lopez-Real JM, Swift JM (1975) The formation of pseudosclerotia (‘zone lines’) in wood decayed byArmillaria melleaandStereum hirsutum,II. Formation in relation to the moisture content of the wood. Trans Br Mycol Soc 64:473–481 Lopez-Real JM, Swift JM (1977) Formation of pseudosclerotia (‘zone lines’) in
wood decayed byArmilllaria melleaandStereum hirsutum,III. Formation in relation to composition of gaseous atmosphere in wood. Trans Br Mycol Soc 68:321–325
Margalith PZ (ed) (1992) Pigment Microbiology. Chapman & Hall Publ, New York Miller VV (1932) Points in the Biological Diagnosis of House Fungi I. The rotting
process as a source of self-wetting for timber. Leningrad State Forestal Technical Publishing Office, Leningrad
Nicholls D (2002)) Evaluation of the retail market potential for Locally Produced Paper Borch Lumber in Alaska. In: General Technical Report PNW-GTR-493. USDA Forest Serv., Pacific Northwest Res. Sta, Portland, OR
Pearce RB (1991) Reaction zone relics and the dynamics of fungal spread in the xylem of woody angiosperms. Phys Mol Plant Pathol 39:41–55
Rayner ADM (1986) Water and the origins of decay in trees. In: Ayrcs PG, Boddy L (eds) Water, fungi and plants. Univ Press, Cambridge, p 32l
Rayner ADM, Todd NK (1979) Population and community structure and dynamics of fungi in decaying wood. Adv Bot Res 7:333–420
Rishbeth J (1951) Observation on the biology ofFomes annosuswith particular reference to East Anglican pine plantations. II. Spore production, stump infection and saprophytic activity in stump. Ann Bot 15:1–21
Robinson SC, Richter DL, Laks PE (2007) Colonization of sugar maple by spalting fungi. For Prod J 57(4):24–32
Robinson SC, Laks PE, Turnquist EJ (2009) A method for digital color analysis of spalted wood using Scion Image software. Materials 2:62–75
Robinson SC, Tudor D, Cooper PA (2012) Promoting fungal pigment formation in wood by utilizing a modified decay jar method. Wood Sci Technol 46:841–849
Rowell RM (2012) Moisture Properties. In: Rowell RM (ed) Handbook of Wood Chemistry and Wood Composites, 2nd edn. CRC Press, New York Taylor R, Dashek WV, Williams AL, Llewellyn GC, Shortle WC, O'Rear CE, Mayficid
JE (1988) Ultrastructure of the wood-decay fungus,Coriolus versicolor,in relation to a catechol-induced bimodal growth response. Int Biodet 24:343–358
Schmidt O (ed) (2006) Wood and tree fungi. Springer-Verlag, Berlin